Materials Science and Engineering An Introduction (9th EDITION) by William D. Callister, Jr & David G. Rethwisch

October 20, 2017 | Author: Fadi Freiga | Category: Logarithm, Diffusion, Density, Equations, Kilogram

ch05 solution...

Description

seCHAPTER 5 DIFFUSION PROBLEM SOLUTIONS

Introduction 5.1 Briefly explain the difference between self-diffusion and interdiffusion. Answer Self-diffusion is atomic migration in pure metals--i.e., when all atoms exchanging positions are of the same type. Interdiffusion is diffusion of atoms of one metal into another metal.

5.2 Self-diffusion involves the motion of atoms that are all of the same type; therefore, it is not subject to observation by compositional changes, as with interdiffusion. Suggest one way in which self-diffusion may be monitored. Answer Self-diffusion may be monitored by using radioactive isotopes of the metal being studied. The motion of these isotopic atoms may be detected by measurement of radioactivity level.

Diffusion Mechanisms 5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Answer (a) With vacancy diffusion, atomic motion is from one lattice site to an adjacent vacancy. Self-diffusion and the diffusion of substitutional impurities proceed via this mechanism. On the other hand, atomic motion is from interstitial site to adjacent interstitial site for the interstitial diffusion mechanism. (b) Interstitial diffusion is normally more rapid than vacancy diffusion because: (1) interstitial atoms, being smaller, are more mobile; and (2) the probability of an empty adjacent interstitial site is greater than for a vacancy adjacent to a host (or substitutional impurity) atom.

5.4 Carbon diffuses in iron via an interstitial mechanism—for FCC iron from one octahedral site to an 1

adjacent one. In Section 4.3 (Figure 4.3a), we note that two general sets of point coordinates for this site are

0 1 2

111

and 2 2 2 . Specify the family of crystallographic directions in which this diffusion of carbon in FCC iron takes place. Solution Below is shown a schematic FCC unit cell, and in addition representations of interstitial atoms located in 1

both

0 1 2

11 1

and

22 2

octahedral sites. In addition, arrows have been drawn from each of these atoms to a nearest

octahedral site: from

1 2

0 1

to

1 11 2 ,

and from

11 1 22 2

to

10

1 2.

(Note: These point coordinates are referenced to the

coordinate system having its origin located at the center of the bottom, rear atom, the one labeled with an O.)

Using the procedure detailed in Section 3.9 for determining the crystallographic direction of a vector (i.e.,

subtraction of vector tail coordinates from head coordinates) coordinates for the 1

x coordinate:

y coordinate:

2

1

0=

2

1

1

2

z coordinate: 1  1 = 0

1 2

1

1

2

2

0 1 to 11

vector are as follows:

In order to reduce these coordinates to integers it is necessary to multiply each by the factor "2". Therefore, this vector points in a [110] direction. 11 1

Applying this same procedure to the x coordinate: y coordinate:

1 

1

0 

1

1

z coordinate:

2

=

2

2 1 2

22 2

to

10

1 2

vector we obtain the following:

1 2

 

1 2

0

Again, multiplying these indices by 2 leads to the [1 10] direction. Therefore, the family of crystallographic directions for the diffusion of interstitial atoms in FCC metals is 110.

5.5   Carbon diffuses in iron via an interstitial mechanism—for BCC iron from one tetrahedral site to an 11

1

adjacent one.  In Section 4.3 (Figure 4.3b) we note that a general set of point coordinates for this site are  2 4 . Specify the family of crystallographic directions in which this diffusion of carbon in BCC iron takes place. Solution Below is shown a schematic BCC unit cell, and in addition the representation of an interstitial atom located

in a

1

1

1 1

tetrahedral site. In addition, an arrow has been drawn from this atom to a nearest tetrahedral site: from

2 4

1 1

1

2 4

2

to

1

1 4

. (Note: These point coordinates are referenced to the coordinate system having its origin located at

the center of the bottom, rear atom, the one labeled with an O.)

Using the procedure detailed in Section 3.9 for determining the crystallographic direction of a vector (i.e.,

subtraction of vector tail coordinates from head coordinates) coordinates for this x coordinate: y coordinate: z coordinate:

1 2

 1 

1 1 4

1 2

1 4

1 2 1 2

=0

1

1 1 2 4

to

1 1 1 2 4

vector are as follows:

In order to reduce these coordinates to integers it is necessary to multiply each by the factor "2". Therefore, this vector points in a [110] direction. Thus, the family of crystallographic directions for the diffusion of interstitial atoms in BCC metals is 110.

Fick's First Law 5.6 Briefly explain the concept of steady state as it applies to diffusion. Answer Steady-state diffusion is the situation wherein the rate of diffusion into a given system is just equal to the rate of diffusion out, such that there is no net accumulation or depletion of diffusing species--i.e., the diffusion flux is independent of time.

5.7 (a) Briefly explain the concept of a driving force. (b) What is the driving force for steady-state diffusion? Answer (a) The driving force is that which compels a reaction to occur. (b) The driving force for steady-state diffusion is the concentration gradient.

5.8 The purification of hydrogen gas by diffusion through a palladium sheet was discussed in Section 5.3. Compute the number of kilograms of hydrogen that pass per hour through a 6-mm thick sheet of palladium having an area of 0.25 m2 at 600°C. Assume a diffusion coefficient of 1.7 × 10–8 m2/s, that the respective concentrations at the high- and low-pressure sides of the plate are 2.0 and 0.4 kg of hydrogen per cubic meter of palladium, and that steady-state conditions have been attained. Solution This problem calls for the mass of hydrogen, per hour, that diffuses through a Pd sheet. It first becomes necessary to employ both Equations 5.1 and 5.2. Combining these expressions and solving for the mass yields

M = J At =  DAt

C x  0.4  2.0 kg/m 3 

=  (1.7  108 m 2 /s)(0.25 m 2 ) (3600 s/h)  

 4.1  10 3 kg/h

6  103 m 

5.9 A sheet of steel 2.5-mm thick has nitrogen atmospheres on both sides at 900°C and is permitted to achieve a steady-state diffusion condition. The diffusion coefficient for nitrogen in steel at this temperature is 1.85 × 10–10 m2/s, and the diffusion flux is found to be 1.0 × 10 –7 kg/m2 . s. Also, it is known that the concentration of nitrogen in the steel at the high-pressure surface is 2 kg/m 3. How far into the sheet from this high-pressure side will the concentration be 0.5 kg/m3? Assume a linear concentration profile. Solution This problem is solved by using Equation 5.2 in the form

J =  D

CA  CB xA  xB

If we take CA to be the point at which the concentration of nitrogen is 2 kg/m 3, then it becomes necessary to solve the above equation for xB, as

 CA  CB   J  

xB = xA + D  Assume xA is zero at the surface, in which case

 2 kg/m 3  0.5 kg/m 3 

xB = 0 + (1.85  1010 m 2 /s) 

 1.0  107 kg/m 2 -s 

 2.78  10 3 m  2.78 mm

5.10 A sheet of BCC iron 2-mm thick was exposed to a carburizing gas atmosphere on one side and a decarburizing atmosphere on the other side at 675°C. After reaching steady state, the iron was quickly cooled to room temperature. The carbon concentrations at the two surfaces of the sheet were determined to be 0.015 and 0.0068 wt%, respectively. Compute the diffusion coefficient if the diffusion flux is 7.36 × 10 –9 kg/m2.s. Hint: Use Equation 4.9 to convert the concentrations from weight percent to kilograms of carbon per cubic meter of iron. Solution Let us first convert the carbon concentrations from weight percent to kilograms carbon per meter cubed using Equation 4.9a; the densities of carbon and iron are 2.25 g/cm3 and 7.87 g/cm3. For 0.015 wt% C

CC =

CC  103 CC CFe  C  Fe

0.015

=

0.015 2.25 g/cm 3

99.985

 103

7.87 g/cm 3

1.18 kg C/m3 Similarly, for 0.0068 wt% C

CC =

0.0068  103 0.0068 99.9932  2.25 g/cm 3 7.87 g/cm3

= 0.535 kg C/m3 Now, using a rearranged form of Equation 5.2

D= J

 x  xB  x = J  A  C  CA  CB 

and incorporating values of plate thickness and diffusion flux, provided in the problem statement, as well as the two concentrations of carbon determined above, the diffusion coefficient is computed as follows:

2  103 m

D=  (7.36  10-9 kg/m 2 -s) 

3

3

 0.535 kg/m  1.18 kg/m 

11

= 2.3  10

m2/s

5.11 When α-iron is subjected to an atmosphere of nitrogen gas, the concentration of nitrogen in the iron, CN (in weight percent), is a function of hydrogen pressure, pN (in MPa), and absolute temperature (T) according to 2

 37, 600 J/mol  CN  4.90  10 3 pN exp    2   RT

(5.14)

Furthermore, the values of D0 and Qd for this diffusion system are 5.0 × 10–7 m2/s and 77,000 J/mol, respectively. Consider a thin iron membrane 1.5-mm thick that is at 300°C. Compute the diffusion flux through this membrane if the nitrogen pressure on one side of the membrane is 0.10 MPa (0.99 atm) and that on the other side is 5.0 MPa (49.3 atm). Solution This problems asks for us to compute the diffusion flux of nitrogen gas through a 1.5-mm thick plate of iron at 300C when the pressures on the two sides are 0.10 and 5.0 MPa. Ultimately we will employ Equation 5.2 to solve this problem. However, it first becomes necessary to determine the concentration of hydrogen at each face using Equation 5.14. At the low pressure (or B) side

  37,600 J/mol CN (B) = (4.90  103 ) 0.10 MPa exp    (8.31 J/mol-K)(300  273 K)   7

5.77  10

wt%

Whereas, for the high pressure (or A) side

  37,600 J/mol CN (A) = (4.90  103 ) 5.0 MPa exp    (8.31 J/mol-K)(300  273 K)   6

4.08  10

wt%

We now convert concentrations in weight percent to mass of nitrogen per unit volume of solid. At face B there are 7

5.77  10

10

g (or 5.77  10

kg) of hydrogen in 100 g of Fe, which is virtually pure iron. From the density of iron

(7.87 g/cm3), the volume iron in 100 g (VB) is just

VB =

100 g 7.87 g/cm

3

= 12.7 cm 3 = 1.27  10-5 m 3

C Therefore, the concentration of hydrogen at the B face in kilograms of N per cubic meter of alloy [ N(B) ] is just

CN(B)  =

=

5.77  10 10 kg 1.27  105 m3

CN(B) VB

= 4.54  10-5 kg/m 3 5

At the A face the volume of iron in 100 g (VA) will also be 1.27  10

CN(A) = 

=

4.08  109 kg 1.27  105 m 3

m3, and

CN(A) VA

= 3.21  10 4 kg/m 3

Thus, the concentration gradient is just the difference between these concentrations of nitrogen divided by the thickness of the iron membrane; that is

  CN(A)  C CN(B) = x xB  xA =

4.54  105 kg/m 3  3.21  104 kg/m 3 1.5  103 m

=  0.184 kg/m 4

At this time it becomes necessary to calculate the value of the diffusion coefficient at 300C using Equation 5.8. Thus,

 Q  D = D0 exp   d   RT    77,000 J/mol = (5.0  107 m 2 /s) exp    (8.31 J/mol-K)(300  273 K)   14

= 4.74  10

m2/s

And, finally, the diffusion flux is computed using Equation 5.2 by taking the negative product of this diffusion coefficient and the concentration gradient, as

J =D



C x

=  ( 4.74  1014 m 2 /s)(  0.184 kg/m 4 ) = 8.72  1015 kg/m 2 -s

Fick's Second Law—Nonsteady-State Diffusion 5.12 Show that

Cx 

 B x2  exp    Dt  4Dt

is also a solution to Equation 5.4b. The parameter B is a constant, being independent of both x and t. Hint: from Equation 5.4b, demonstrate that

 B x2   exp    Dt  4Dt   t

 

is equal to



 2  D  

 B x2    exp     Dt  4Dt    

x2

 

Solution When these differentiations are carried out, both are equal to the following expression:

 x2   1 exp  2 D1/2t3/2  2 Dt 

B

 

x2   4 Dt 

5.13 Determine the carburizing time necessary to achieve a carbon concentration of 0.30 wt% at a position 4 mm into an iron–carbon alloy that initially contains 0.10 wt% C. The surface concentration is to be maintained at 0.90 wt% C, and the treatment is to be conducted at 1100°C. Use the diffusion data for γ-Fe in Table 5.2. Solution We are asked to compute the carburizing (i.e., diffusion) time required for a specific nonsteady-state diffusion situation. It is first necessary to use Equation 5.5:

Cx  C0  x  = 1  erf  Cs  C0  2 Dt   3

wherein, Cx = 0.30, C0 = 0.10, Cs = 0.90, and x = 4 mm = 4  10

m. Thus,

Cx  C0 0.30  0.10  x  = = 0.2500 = 1  erf  Cs  C0 0.90  0.10  2 Dt   or

 x  erf  = 1  0.2500 = 0.7500  2 Dt   By linear interpolation using data from Table 5.1 z

erf(z)

0.80

0.7421

z

0.7500

0.85

0.7707

which leads to the following:

z  0.800 0.7500  0.7421 = 0.850  0.800 0.7707  0.7421 From which

z = 0.814 =

x 2 Dt

Now, from Table 5.2, data for the diffusion of carbon into -iron are as follows: D0 = 2.3 105 m2/s

Qd = 148,000 J/mol Therefore at 1100C (1373 K)

  148,000 J/mol D = (2.3  10-5 m 2 /s) exp     (8.31 J/mol-K)(1373 K)  11

= 5.35  10

m2/s

Thus,

4  103 m

0.814 = (2)

(5.35  1011 m 2 /s) (t)

Solving for t yields

t

(4  10 3 m)2

(2)2 (0.814)2 (5.35  10 11 m 2 /s) t = 1.13  105 s = 31.3 h

5.14 An FCC iron–carbon alloy initially containing 0.55 wt% C is exposed to an oxygen-rich and virtually carbon-free atmosphere at 1325 K (1052°C). Under these circumstances the carbon diffuses from the alloy and reacts at the surface with the oxygen in the atmosphere—that is, the carbon concentration at the surface position is maintained essentially at 0 wt% C. (This process of carbon depletion is termed decarburization.) At what position will the carbon concentration be 0.25 wt% after a 10-h treatment? The value of D at 1325 K is 3.3 × 10–11 m2/s. Solution This problem asks that we determine the position at which the carbon concentration is 0.25 wt% after a 10h heat treatment at 1325 K when C0 = 0.55 wt% C. From Equation 5.5

Cx  C0  0.25  0.55 x  = = 0.5455 = 1  erf  Cs  C0 0  0.55  2 Dt   Thus,

 x  erf  = 0.4545  2 Dt   Using data in Table 5.1 and linear interpolation z

erf (z)

0.40

0.4284

z

0.4545

0.45

0.4755

z  0.40 0.4545  0.4284 = 0.45  0.40 0.4755  0.4284 which leads to,



z = 0.4277

This means that

x 2 Dt

= 0.4277

And, finally

x = 2(0.4277) Dt= (0.8554)

(3.3  1011 m 2 /s)( 3.6  104 s)

4

= 9.32  10

m = 0.932 mm

Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “Diffusion Design” submodule, and then do the following: 1. Enter the given data in left-hand window that appears. In the window below the label “D Value” enter the value of the diffusion coefficient—viz. “3.3e-11”. 2. In the window just below the label “Initial, C0” enter the initial concentration—viz. “0.55”. 3. In the window the lies below “Surface, Cs” enter the surface concentration—viz. “0”. 4. Then in the “Diffusion Time t” window enter the time in seconds; in 10 h there are (60 s/min)(60 min/h) (10 h) = 36,000 s—so enter the value “3.6e4”. 5. Next, at the bottom of this window click on the button labeled “Add curve”. 6. On the right portion of the screen will appear a concentration profile for this particular diffusion situation. A diamond-shaped cursor will appear at the upper left-hand corner of the resulting curve. Click and drag this cursor down the curve to the point at which the number below “Concentration:” reads “0.25 wt%”. Then read the value under the “Distance:”. For this problem, this value (the solution to the problem) is 0.91 mm.

5.15 Nitrogen from a gaseous phase is to be diffused into pure iron at 675°C. If the surface concentration is maintained at 0.2 wt% N, what will be the concentration 2 mm from the surface after 25 h? The diffusion coefficient for nitrogen in iron at 675°C is 2.8 × 10–11 m2/s. Solution This problem asks us to compute the nitrogen concentration (Cx) at the 2 mm position after a 25 h diffusion time, when diffusion is nonsteady-state. From Equation 5.5

Cx  C0 C 0  x  = x = 1  erf  Cs  C0 0.2  0  2 Dt     (2) 

( 2.8  1011 m 2 /s) (25 h)(3600 s/h)  = 1 – erf (0.630)

Using data in Table 5.1 and linear interpolation z

erf (z)

0.600

0.6039

0.630

y

0.650

0.6420

0.630  0.600 y  0.6039 = 0.650  0.600 0.6420  0.6039 from which y = erf (0.630) = 0.6268 Thus,

Cx  0 = 1.0  0.6268 0.2  0 And solving for Cx gives

2  103 m

= 1  erf 

Cx = 0.075 wt% N Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “Diffusion Design” submodule, and then do the following: 1. Enter the given data in left-hand window that appears. In the window below the label “D Value” enter the value of the diffusion coefficient—viz. “2.8e-11”. 2. In the window just below the label “Initial, C0” enter the initial concentration—viz. “0”. 3. In the window the lies below “Surface, Cs” enter the surface concentration—viz. “0.2”. 4. Then in the “Diffusion Time t” window enter the time in seconds; in 25 h there are (60 s/min)(60 min/h) (25 h) = 90,000 s—so enter the value “9e4”. 5. Next, at the bottom of this window click on the button labeled “Add curve”. 6. On the right portion of the screen will appear a concentration profile for this particular diffusion situation. A diamond-shaped cursor will appear at the upper left-hand corner of the resulting curve. Click and drag this cursor down the curve to the point at which the number below “Distance:” reads “2.00 mm”. Then read the value under the “Concentration:”. For this problem, this value (the solution to the problem) is 0.07 wt%.

5.16 Consider a diffusion couple composed of two semi-infinite solids of the same metal and that each side of the diffusion couple has a different concentration of the same elemental impurity; furthermore, assume each impurity level is constant throughout its side of the diffusion couple. For this situation, the solution to Fick’s second law (assuming that the diffusion coefficient for the impurity is independent of concentration) is as follows:

x     C1  C2    1 erf    2   2 Dt  

Cx  C2  

(5.15)

The schematic diffusion profile in Figure 5.13 shows these concentration parameters as well as concentration profiles at times t = 0 and t > 0. Please note that at t = 0, the x = 0 position is taken as the initial diffusion couple interface, whereas C1 is the impurity concentration for x < 0, and C2 is the impurity content for x > 0. Consider a diffusion couple composed of pure nickel and a 55 wt% Ni-45 wt% Cu alloy (similar to the couple shown in Figure 5.1). Determine the time this diffusion couple must be heated at 1000°C (1273 K) in order to achieve a composition of 56.5 wt% Ni a distance of 15 μm into the Ni-Cu alloy referenced to the original interface. Values for the preexponential and activation energy for this diffusion system are 2.3  10-4 m2/s and 252,000 J/mol. Solution This problem calls for us to determine the value of time t in Equation 5.15 given the following values: C1 = 100 wt% Ni C2 = 55 wt% Ni Cx = 56.5 wt% Ni T = 1273 K x = 15 μm = 15  10-6 m D0 = 2.3  10-4 m2/s Qd = 252,000 J/mol

Let us first of all compute the value of the diffusion coefficient D using Equation 5.8:

 Q  D  D0 exp   d   RT 

  252,000 J/mol  (2.3  104 m 2 /s)exp     (8.31 J/moliK)(1273 K) 

 1.04  1014 m 2 /s Now incorporating values for all of the parameters except t into Equation 5.12 leads to

     100 wt% Ni  55 wt% Cu   15  106 m   1  erf   2    2 (1.04  1014 m 2 /s)( t)    

56.5 wt% Ni  55 wt% Ni +  

This expression reduces to the following:

 73.54 s1/2 

0.9333  erf  

 

t

From Table 5.1 to determine the value of z when erf(z) = 0.9333 an interpolation procedure is necessary as follows:

z

erf(z)

1.2

0.9103

z

0.9333

1.3

0.9340

z  1.2 0.9333  0.9103  1.3  1.2 0.9340  0.9103

And solving for z we have z = 1.297 Which means that

73.54 s1/2 t

 1.297

Or that 2

 73.54 1/2  t s   1.297 

 3215 s = 53.6 min  0.89 h

5.17 Consider a diffusion couple composed of two cobalt-iron alloys; one has a composition of 75 wt% Co-25 wt% Fe; the other alloy composition is 50 wt% Co-50 wt% Fe. If this couple is heated to a temperature of 800°C (1073 K) for 20,000 s, determine how far from the original interface into the 50 wt% Co-50 wt% Fe alloy the composition has increased to 52 wt%Co-48 wt% Fe. For the diffusion coefficient, assume values of 6.6  10-6 m2/s and 247,000 J/mol, respectively, for the preexponential and activation energy. Solution

This problem calls for us to determine the value of the distance, x, in Equation 5.15 given the following values: C1 = 75 wt% Co C2 = 50 wt% Co Cx = 52 wt% Co T = 1073 K t = 20,000 s D0 = 6.6  10-6 m2/s Qd = 247,000 J/mol

Let us first of all compute the value of the diffusion coefficient D using Equation 5.8:

 Q  D  D0 exp   d   RT 

  247,000 J/mol  (6.6  106 m 2 /s)exp     (8.31 J/moliK)(1073 K) 

 6.15  1018 m 2 /s Now incorporating values for all of the parameters except x into Equation 5.15 leads to

     75 wt% Co  50 wt% Co   x   52 wt% Co  50 wt% Co +  1  erf   2     2 (6.15  1018 m 2 /s)( 20,000 s)     This expression reduces to the following:

x  7.01 

107

0.8400  erf 

m

From Table 5.1 to determine the value of z when erf(z) = 0.8400 an interpolation procedure is necessary as follows:

z

erf(z)

0.95

0.8209

z

0.8400

1.0

0.8427

z  0.95 0.8400  0.8209  1.0  0.95 0.8427  0.8209 And solving for z we have z = 0.994 Which means that

x 7.01  107 m

 0.994

Or that

x  (7.01  107 m)(0.994)  6.97  107 m  0.697 m

5.18 Consider a diffusion couple between silver and a gold alloy that contains 10 wt% silver. This couple is heat treated at an elevated temperature and it was found that after 850 s the concentration of silver had increased to 12 wt% at 10 μm from the interface into the Ag-Au alloy. Assuming preexponential and activation energy values of 7.2  10-6 m2/s and 168,000 J/mol, compute the temperature of this heat treatment. (Note: you may find Figure 5.13 and Equation 5.15 helpful.) Solution

This problem calls for us to determine the value of time t in Equation 5.15 given the following values: C1 = 100 wt% Ag C2 = 10 wt Ag Cx = 12 wt% Ag t = 850 s x = 10 μm = 10  10-6 m D0 = 7.2  10-6 m2/s Qd = 168,000 J/mol We first of all substitute values for all of the above parameters—except for D0 and Qd. This leads to the following expressions:

 C1  C2    x    1  erf    2    2 Dt    

C x  C2 + 

 10  106 m    100 wt%  10 wt%    1  erf    2   2 D(850 s)    

12 wt%  10 wt% +   This equation reduces to the following:

 1.715  107 

0.9556  erf  

D

Or

 

0.9556  erf z

It is now necessary to determine using the data in Table 5.1 the value of z for which the error function has a value of 0.9556. This requires an interpolation using the following data:

z

erf(z)

1.4

0.9523

z

0.9556

1.5

0.9661

The interpolation equation is

1.5  z 0.9661  0.9556  1.5  1.4 0.9661  0.9523 Solving for z from this equation gives z =1.424 Incorporating this value into the above equation yields

1.424 

1.715  107 D

from which D is equal to

D  1.45  1014 m 2 /s We may now compute the temperature at which the diffusion coefficient has this value using Equation 5.8. Taking natural logarithms of both sides of Equation 5.8 leads to

ln D  ln D0 

Qd RT

And, solving for T

T= 

Qd R(ln D  ln D0 )

Into which we insert values of D, D0, and Qd as follows:

T= 

168,000 J/m  (8.31 J/mol K) ln (1.45  1014 m 2 /s)  ln (7.2  106 m 2 /s)    = 1010 K (737C)

5.19 For a steel alloy it has been determined that a carburizing heat treatment of 15 h duration will raise the carbon concentration to 0.35 wt% at a point 2.0 mm from the surface. Estimate the time necessary to achieve the same concentration at a 6.0-mm position for an identical steel and at the same carburizing temperature. Solution

This problem calls for an estimate of the time necessary to achieve a carbon concentration of 0.35 wt% at a point 6.0 mm from the surface. From Equation 5.6b,

x2 = constant Dt But since the temperature is constant, so also is D constant, which means that

x2 = constant t or

x12 x22 = t1 t2 Thus, if we assign x1 = 0.2 mm, x2 = 0.6 mm, and t1 15 h, then

(2.0 mm) 2 (6.0 mm) 2 = 15 h t2 from which



t2 = 135 h

Factors That Influence Diffusion 5.20 Cite the values of the diffusion coefficients for the interdiffusion of carbon in both α-iron (BCC) and γ-iron (FCC) at 900°C. Which is larger? Explain why this is the case. Solution

We are asked to compute the diffusion coefficients of C in both  and  iron at 900C. Using the data in Table 5.2,

  87,400 J/mol D = (1.1  10-6 m 2 /s) exp     (8.31 J/mol-K)(1173 K) 

 1.40  1010 m 2 /s

  148,000 J/mol D = (2.3  105 m 2 /s) exp     (8.31 J/mol-K)(1173 K) 

 5.86  10 12 m 2 /s The D for diffusion of C in BCC  iron is larger, the reason being that the atomic packing factor is smaller than for FCC  iron (0.68 versus 0.74—Section 3.4); this means that there is slightly more interstitial void space in the BCC Fe, and, therefore, the motion of the interstitial carbon atoms occurs more easily.

5.21 Using the data in Table 5.2, compute the value of D for the diffusion of magnesium in aluminum at 400°C. Solution This problem asks us to compute the magnitude of D for the diffusion of Mg in Al at 400C (673 K). Incorporating the appropriate data from Table 5.2—i.e., D0 = 1.2  104 m2/s Qd = 130,000 J/mol into Equation 5.8 leads to

 Q  D  D0 exp   d   RT    130,000 J/mol = (1.2  104 m 2 /s) exp     (8.31 J/mol-K)(673 K) 

 9.64  1015 m 2 /s Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D vs 1/T Plot” submodule, and then do the following: 1. In the left-hand window that appears, click on the “Mg-Al” pair under the “Diffusing Species”-“Host Metal” headings. 2. Next, at the bottom of this window, click the “Add Curve” button. 3. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for Mg in Al. At the top of this curve is a diamond-shaped cursor. Click-and-drag this cursor down the line to the point at which the entry under the “Temperature (T):” label reads 673 K (inasmuch as this is the Kelvin equivalent of 400ºC). Finally, the diffusion coefficient value at this temperature is given under the label “Diff Coeff  (D):”. For this problem, the value is 8.0  10 15 m2/s.

5.22 Using the data in Table 5.2 compute the value of D for the diffusion of nitrogen in FCC iron at 950C. Solution This problem asks us to compute the magnitude of D for the diffusion of N in FCC Fe at 950C. Incorporating the appropriate data from Table 5.2—i.e., D0 = 9.1  105 m2/s Qd = 168,000 J/mol into Equation 5.8 leads to

 Q  D  D0 exp   d   RT    168,000 J/mol = (9.1  105 m 2 /s) exp     (8.31 J/mol-K)(950C  273) 

 6.0  10 12 m 2 /s Note: this problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D vs 1/T Plot” submodule, and then do the following: 1. In the left-hand window that appears, click on the "Custom 1 under the “Diffusing Species” heading (since none of the preset systems is for the diffusion of nitrogen in FCC iron). 2. Under "D0" within the "Diffusion Coefficients" box enter "9.1e-5"; and under "Qd" enter "168". 3. It is necessary to enter maximum and minimum temperatures within the "Temperature Range" box. Because our temperature of interest is 950C, enter "900" in the "T Min" "C" box, and "1000" in the T Max "C" box. 3. Upon clicking on the "Add Curve" box, a log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for N in FCC iron. At the top of this curve is a diamond-shaped cursor. Click-and-drag this cursor down the line to the point at which the entry under the “Temperature (T):” label reads 1223 K (inasmuch as this is the Kelvin equivalent of 950ºC). Finally, the diffusion coefficient value at this  temperature is given under the label “Diff Coeff (D):”. For this problem, the value is 6.0  10 12 m2/s.

5.23 At what temperature will the diffusion coefficient for the diffusion of zinc in copper have a value of 2.6 × 10

–16

m2/s? Use the diffusion data in Table 5.2. Solution

We are asked to calculate the temperature at which the diffusion coefficient for the diffusion of Zn in Cu 16

has a value of 2.6  10

m2/s. Solving for T from Equation 5.9a

T= 

Qd R(ln D  ln D0 )

and using the data from Table 5.2 for the diffusion of Zn in Cu (i.e., D0 = 2.4  10

5

m2/s and Qd = 189,000 J/mol) ,

we get

T= 

189,000 J/mol (8.31 J/mol-K)  ln (2.6  10 16 m 2 /s)  ln (2.4  10 5 m 2 /s)    = 901 K = 628C

Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D vs 1/T Plot” submodule, and then do the following: 1. In the left-hand window that appears, there is a preset set of data for the diffusion of Zn in Cu system. Therefore, click on the "Cu-Ni" box. 2. In the column on the right-hand side of this window the activation energy-preexponential data for this problem. In the window under “D 0” the preexponential value, “2.4e-5”, is displayed. Next just below the “Q d” the activation energy value (in KJ/mol), “189” is displayed. In the "Temperature Range" window minimum ("T Min") and maximum ("T Max") temperatures are displayed, in both C and K. The default values for minimum and maximum temperatures are 800ºC and 1140ºC, respectively. 3. Next, at the bottom of this window, click the "Add Curve" button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for Zn in Cu. At the top of this curve is a diamond-shaped cursor. We want to click-and-drag this cursor down the line (to the right) to the point at which the entry under the “Diff Coeff (D):” label reads 2.6  10-16 m2/s.

As we drag the cursor to the right, the value of the diffusion coefficient continues to decrease, but only to about 1.5  10-14 m2/s. This means that the temperature at which the diffusion coefficient is 2.6  10-16 m2/s is lower than 800ºC. Therefore, let us change the T Min value to 600ºC. After this change is made click again on the "Add Curve", and a new curve appears. Now click and drag the cursor to the right until "2.6  10-16 m2/s " is displayed under "Diff Coeff (D)". At this time under the "Temperature (T)" label is displayed the temperature—in this case "902 K".

5.24 At what temperature will the diffusion coefficient for the diffusion of nickel in copper have a value of 4.0  10-17 m2/s? Use the diffusion data in Table 5.2. Solution We are asked to calculate the temperature at which the diffusion coefficient for the diffusion of Ni in Cu 17

has a value of 4.0  10

m2/s. Solving for T from Equation 5.9a

T= 

Qd R(ln D  ln D0 )

and using the data from Table 5.2 for the diffusion of Ni in Cu (i.e., D0 = 1.9  10

4

m2/s and Qd = 230,000 J/mol) ,

we get

T= 

230,000 J/mol (8.31 J/mol-K)  ln (4.0  10 17 m 2 /s)  ln (1.9  10 4 m 2 /s)    = 948 K = 675C

Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D vs 1/T Plot” submodule, and then do the following: 1. In the left-hand window that appears, there is a preset set of data, but none for the diffusion of Ni in Cu. This requires us specify our settings by clicking on the “Custom1” box. 2. In the column on the right-hand side of this window enter the data for this problem, which are taken from Table 5.2. In the window under “D0” the preexponential value, enter “1.9e-4”. Next just below in the “Q d” window enter the activation energy value (in KJ/mol), in this case "230". It is now necessary to specify a temperature range over which the data is to be plotted—let us arbitrarily pick 500 C to be the miminum, which is entered in the "T Min" under "Temperature Range" window; we will also select 1000C to be the maximum temperature, which is entered in the "T Max" window. 3. Next, at the bottom of this window, click the "Add Curve" button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for Ni in Cu. At the top of this curve is a diamond-shaped cursor. We next click-and-drag this cursor

down the line to the point at which the entry under the “Diff Coeff (D):” label reads 4.0  10-17 m2/s. The temperature that appears under the "Temperature (T)" label is 949 K, which is the solution.

5.25 The preexponential and activation energy for the diffusion of chromium in nickel are 1.1 × 10 –4 m2/s and 272,000 J/mol, respectively. At what temperature will the diffusion coefficient have a value of 1.2 × 10 –14 m2/s? Solution We are asked to calculate the temperature at which the diffusion coefficient for the diffusion of Cr in Ni has 14

a value of 1.2  10

m2/s. Solving for T from Equation 5.9a

T= 

Qd R(ln D  ln D0 ) 4

and using the data the problem statement (i.e., D0 = 1.1  10

T= 

m2/s and Qd = 272,000 J/mol) , we get

272,000 J/mol (8.31 J/mol-K)  ln (1.2  10 14 m 2 /s)  ln (1.1  10 4 m 2 /s)    = 1427 K = 1154C

Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D vs 1/T Plot” submodule, and then do the following: 1. In the left-hand window that appears, there is a preset set of data, but none for the diffusion of Cr in Ni. This requires us specify our settings by clicking on the “Custom1” box. 2. In the column on the right-hand side of this window enter the data for this problem, which are given in the problem statement. In the window under “D 0” enter “1.1e-4”. Next just below in the “Q d” window enter the activation energy value (in KJ/mol), in this case "272". It is now necessary to specify a temperature range over which the data is to be plotted—let us arbitrarily pick 1000C to be the miminum, which is entered in the "T Min" under "Temperature Range" window; we will also select 1500C to be the maximum temperature, which is entered in the "T Max" window. 3. Next, at the bottom of this window, click the "Add Curve" button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for Cr in Ni. At the top of this curve is a diamond-shaped cursor. We next click-and-drag this cursor

down the line to the point at which the entry under the “Diff Coeff (D):” label reads 1.2  10-14 m2/s. The temperature that appears under the "Temperature (T)" label is 1430 K.

5.26 The activation energy for the diffusion of copper in silver is 193,000 J/mol. Calculate the diffusion coefficient at 1200 K (927°C), given that D at 1000 K (727°C) is 1.0 × 10–14 m2/s. Solution To solve this problem it first becomes necessary to solve for D0 from a rearranged form of Equation 5.8 and using 1000 K diffusion data:

 Qd    RT 

D0 = D exp  

 193,000 J/mol   (8.31 J/mol-K)(1000 K) 

= (1.0  10 14 m 2 /s) exp 

1.22  10 4 m 2 /s Now, solving for D at 1200 K (again using Equation 5.8) gives

  193,000 J/mol D = (1.22  104 m 2 /s) exp     (8.31 J/mol-K)(1200 K) 

4.8  10 13 m 2 /s

5.27 The diffusion coefficients for nickel in iron are given at two temperatures, as follows: D (m2/s) 2.2 × 10–15 4.8 × 10–14

T (K) 1473 1673

(a) Determine the values of D0 and the activation energy Qd. (b) What is the magnitude of D at 1300°C (1573 K)? Solution (a) Using Equation 5.9a, we set up two simultaneous equations with Qd and D0 as unknowns as follows:

ln D1  ln D0 

Qd  1  R  T1  

ln D2  ln D0 

Qd  1  R  T2  

Now, solving for Qd in terms of temperatures T1 and T2 (1473 K and 1673 K) and D1 and D2 (2.2  10 14

10

m2/s), we get

Qd =  R

ln D1  ln D2 1 1  T1 T2

 ln (2.2  10 15)  ln (4.8  10 14) 

=  (8.31 J/mol-K) 

1 1  1473 K 1673 K

= 315,700 J/mol Now, solving for D0 from a rearranged form of Equation 5.8 (and using the 1473 K value of D)

 Q  D0 = D1 exp  d   RT1  

 315,700 J/mol  (8.31 J/mol-K)(1473 K)  

= (2.2  1015 m 2 /s) exp 

15

and 4.8 

 3.5  10 4 m 2 /s (b) Using these values of D0 and Qd, D at 1573 K is just

  315,700 J/mol D = (3.5  10 4 m 2 /s) exp     (8.31 J/mol-K)(1573 K) 

= 1.1  1014 m 2 /s

Note: This problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D0 and Qd from Experimental Data” submodule, and then do the following: 1. In the left-hand window that appears, enter the two temperatures from the table in the book (viz. “1473” and “1673”, in the first two boxes under the column labeled “T (K)”. Next, enter the corresponding diffusion coefficient values (viz. “2.2e-15” and “4.8e-14”). 3. Next, at the bottom of this window, click the “Plot data” button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence for this diffusion system. At the top of this window are give values for D0 and Qd; for this specific problem these values are 3.49  10-4 m2/s ("Do=3.49E-04") and 315 kJ/mol ("Qd=315"), respectively 5. To solve the (b) part of the problem we utilize the diamond-shaped cursor that is located at the top of the line on this plot. Click-and-drag this cursor down the line to the point at which the entry under the “Temperature (T):” label reads “1573”. The value of the diffusion coefficient at this temperature is given under the label “Diff Coeff (D):”. For our problem, this value is 1.2  10-14 m2/s ("1.2E-14 m2/s").

5.28 The diffusion coefficients for carbon in nickel are given at two temperatures are as follows: D (m2/s) 5.5 × 10–14 3.9 × 10–13

T (°C) 600 700 (a) Determine the values of D0 and Qd. (b) What is the magnitude of D at 850°C? Solution

(a) Using Equation 5.9a, we set up two simultaneous equations with Qd and D0 as unknowns as follows:

ln D1  ln D0 

Qd  1  R  T1  

ln D2  ln D0 

Qd  1  R  T2  

 Solving for Qd in terms of temperatures T1 and T2 (873 K [600C] and 973 K [700C]) and D1 and D2 (5.5  10 14 13

and 3.9  10

m2/s), we get

Qd =  R

= 

ln D1  ln D2 1 1  T1 T2

(8.31 J/mol-K)  ln (5.5  10 14)  ln (3.9  10 13 )    1 1  873 K 973 K = 138,300 J/mol

Now, solving for D0 from a rearranged form of Equation 5.8 (and using the 600C value of D)

 Q  D0 = D1 exp  d   RT1  

 138,300 J/mol   (8.31 J/mol-K)(873 K) 

= (5.5  10 14 m 2 /s) exp 

 1.05  105 m 2 /s (b) Using these values of D0 and Qd, D at 1123 K (850C) is just

  138,300 J/mol D = (1.05  105 m 2 /s) exp     (8.31 J/mol-K)(1123 K) 

 3.8  1012 m 2 /s

Note: this problem may also be solved using the “Diffusion” module in the VMSE software. Open the “Diffusion” module, click on the “D0 and Qd from Experimental Data” submodule, and then do the following: 1. In the left-hand window that appears, enter the two temperatures from the table in the book (converted from degrees Celsius to Kelvins) (viz. “873” (600ºC) and “973” (700ºC), in the first two boxes under the column labeled “T (K)”. Next, enter the corresponding diffusion coefficient values (viz. “5.5e-14” and “3.9e-13”). 3. Next, at the bottom of this window, click the “Plot data” button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence for this diffusion system. At the top of this window are give values for D0 and Qd; for this specific problem these values are 1.04  10-5 m2/s ("Do=1.04E-05") and 138 kJ/mol ("Qd=138"), respectively 5. It is not possible to solve part (b) of this problem using this submodule—data plotted do not extend to 850ºC. Therefore, it necessary to utilize the "D vs 1/T Plot" submodule. 6. Open this submoduile, and in the left-hand window that appears, there is a preset set of data, but none for the diffusion of C in Ni. This requires us specify our settings by clicking on the “Custom1” box. 7. In the column on the right-hand side of this window enter the data for this problem, which have already been determined. In the window under “D 0” the preexponential value, enter “1.04e-5”. Next just below in the “Q d” window enter the activation energy value (in KJ/mol), in this case "138". It is now necessary to specify a temperature range over which the data is to be plotted—since we are interested in the value of D at 850ºC let us arbitrarily pick 600C to be the miminum, which is entered in the "T Min" under "Temperature Range" window; let us also select 900C to be the maximum temperature, which is entered in the "T Max" window.

8. Next, at the bottom of this window, click the "Add Curve" button. 9. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for C in Ni. At the top of this curve is a diamond-shaped cursor. We next click-and-drag this cursor down the line to the point at which the entry under the "Temperature (T)" label reads 1123 K. The value of the diffusion coefficient at this temperature is displayed below the “Diff Coeff (D)” label, which is 3.9  10-12 m2/s.

5.29 The accompanying figure shows a plot of the logarithm (to the base 10) of the diffusion coefficient versus reciprocal of the absolute temperature for the diffusion of gold in silver. Determine values for the activation energy and preexponential.

Solution This problem asks us to determine the values of Qd and D0 for the diffusion of Au in Ag from the plot of Q Q  d  d R since we log D versus 1/T. According to Equation 5.9b the slope of this plot is equal to 2.3 R (rather than are using log D rather than ln D); furthermore, the intercept at 1/T = 0 gives the value of log D0. The slope is equal to

slope =

 (log D) log D1  log D2 = 1 1  1    T1 T2  T

Taking 1/T1 and 1/T2 as 1.0  10-3 and 0.90  10

3

1

K , respectively, then the corresponding values of log D1 and

log D2 are –14.68 and –13.57. Therefore,

Qd =  2.3 R (slope) Qd =  2.3 R

log D1  log D2 1 1  T1 T2 

14.68  (13.57)

=  (2.3)(8.31 J/mol-K) 

 (1.0  103  0.90  10 3 ) K 1 

= 212,200 J/mol Rather than trying to make a graphical extrapolation to determine D0, a more accurate value is obtained analytically using a rearranged form of Equation 5.9b taking a specific value of both D and T (from 1/T) from the    plot given in the problem; for example, D = 1.0  10 14 m2/s at T = 1064 K (1/T = 0.94  10 3 K 1). Therefore

 Qd   RT  

D0 = D exp 

 212,200 J/mol   (8.31 J/mol-K)(1064 K) 

= (1.0  1014 m 2 /s) exp 

 2.65  104 m 2 /s

5.30 The accompanying figure shows a plot of the logarithm (to the base 10) of the diffusion coefficient versus reciprocal of the absolute temperature for the diffusion of vanadium in molybdenum. Determine values for the activation energy and preexponential.

Solution This problem asks us to determine the values of Qd and D0 for the diffusion of V in Mo from the plot of log

Qd Q  d 2.3 R R since we are D versus 1/T. According to Equation 5.9b the slope of this plot is equal to (rather than using log D rather than ln D); furthermore, the intercept at 1/T = 0 gives the value of log D0. The slope is equal to 

slope =

3

Taking 1/T1 and 1/T2 as 0.50  10

 (log D) log D1  log D2 = 1 1  1    T T  T 1 2 3

and 0.55  10

K 1, respectively, then the corresponding values of log D1 and

log D2 are –15.90 and –17.13. Therefore,

Qd =  2.3 R (slope)

Qd =  2.3 R

log D1  log D2 1 1  T1 T2

15.90  (17.13)

=  (2.3)(8.31 J/mol-K) 

 (0.50  103  0.55  103 ) K 1 

= 470,200 J/mol Rather than trying to make a graphical extrapolation to determine D0, a more accurate value is obtained analytically using Equation 5.9b taking a specific value of both D and T (from 1/T) from the plot given in the    problem; for example, D = 1.26  10 16 m2/s at T = 2000 K (1/T = 0.50  10 3 K 1). Therefore

 Qd   RT  

D0 = D exp 

 470,200 J/mol   (8.31 J/mol-K)(2000 K) 

= (1.26  1016 m 2 /s) exp 

 2.44  104 m 2 /s

5.31 From Figure 5.12 calculate activation energy for the diffusion of (a) copper in silicon, and (b) aluminum in silicon (c) How do these values compare? Solution (a) In order to determine the activation energy for the diffusion of copper in silicon, it is necessary to take the slope of its log D versus 1/T curve. The activation energy Qd is equal to the equation cited in Example Problem 5.5—viz.

 log D  log D  1 2 Qd =  2.3R  1 1      T1 T1   On the plot of Figure 5.12, for copper, let us arbitrarily take 1/T1 = 1.5  103 (K1) 1/T2 = 0.6  103 (K1) Their corresponding log D values are log D1 = 9.6 log D2 = 7.7 Thus,

9.6  (  7.7)

Qd =  (2.3)(8.31 J/mol K) 

 1.5 

10 3

K 1

 0.6 

103

 K 1

 40,350 J/mol (b) For aluminum in silicon, let us use the following two log D versus 1/T values: 1/T1 = 1.5  103 (K1) 1/T2 = 0.6  103 (K1) Their corresponding log D values are log D1 = 29.0 log D2 = 13.5

Therefore, the activation energy is equal to

29.0  ( 13.5)  1.5  10

3

Qd =  (2.3)(8.31 J/mol K) 

K

1

 0.6  10

3

K

1 

 330,000 J/mol (c) The activation energy for the diffusion of Al in Si (330,000 J/mol) is approximately eight times the value for the diffusion of Cu in Si (40,350 J/mol).

5.32 Carbon is allowed to diffuse through a steel plate 10 mm thick. The concentrations of carbon at the two faces are 0.85 and 0.40 kg C/cm3 Fe, which are maintained constant. If the preexponential and activation energy are 5.0 × 10–7 m2/s and 77,000 J/mol, respectively, compute the temperature at which the diffusion flux is 6.3 × 10–10 kg/m2.s. Solution This problem asks that we compute the temperature at which the diffusion flux is 6.3  10

10

kg/m2-s.

Combining Equations 5.2 and 5.8 yields

J =D

=  D0

C x

 Q  C exp   d  x  RT 

Taking natural logarithms of both sides of this equation yields the following expression:

 C  Qd ln J  ln  D0  x    RT Or

 D C  Qd  C   ln  D0  ln J  ln   0   RT x  J x    And solving for T from this expression leads to

 Q  1 T =  d  D C   R ln   0  J x   Now, incorporating values of the parameters in this equation provided in the problem statement leads to the following:

 77,000 J/mol  T=  8.31 J/mol-K  

1 

ln   

(5.0 )(0.40 kg/m3  0.85 kg/m3 )   (6.3  1010 kg/m 2 -s)(10  103 m)   107 m 2 /s

= 884 K = 611C

5.33 The steady-state diffusion flux through a metal plate is 7.8 × 10–8 kg/m2.s at a temperature of 1200°C (1473 K) and when the concentration gradient is –500 kg/m4. Calculate the diffusion flux at 1000°C (1273 K) for the same concentration gradient and assuming an activation energy for diffusion of 145,000 J/mol. Solution In order to solve this problem, we must first compute the value of D0 from the data given at 1200C (1473 K); this requires the combining of both Equations 5.2 and 5.8 as

J =D

C x

 Q  C =  D0 exp    d  x   RT   Solving for D0 from the above expression gives

 D0 = 

 Q  J exp  d  C  RT  x

And incorporating values of the parameters in this expressions provided in the problem statement yields the following:

 7.8  108 kg/m 2 -s 

D0 =   

500 kg/m 4

 145,000 J/mol   (8.31 J/mol-K)(1200 + 273 K) 

 exp  

5

= 2.18  10

m2/s

The value of the diffusion flux at 1273 K may be computed using these same two equations as follows:

 Q   C exp   d     x  RT 

J =  D0 

  145,000 J/mol =  ( 2.18  10-5 m 2 /s)(500 kg/m 4 ) exp    (8.31 J/mol-K)(1273 K)   8

= 1.21  10

kg/m2-s

5.34 At approximately what temperature would a specimen of γ-iron have to be carburized for 4 h to produce the same diffusion result as carburization at 1000°C for 12 h? Solution To solve this problem it is necessary to employ Equation 5.7

Dt = constant which, for this problem, takes the form



D1000t1000 = DTtT

At 1000C, and using the data from Table 5.2, for the diffusion of carbon in -iron—i.e., 5

D0 = 2.3  10

m2/s

Qd = 148,000 J/mol the diffusion coefficient is equal to

  148,000 J/mol D1000 = (2.3  105 m 2 /s) exp     (8.31 J/mol-K)(1000  273 K) 

 1.93  1011 m 2 /s Thus, from the above for of Equation 5.7

(1.93

 1011 m 2 /s) (12 h) = DT (4 h)

And, solving for DT

DT =

(1.93  1011

m 2 /s)(12 h) = 5.79  10 11 m 2 /s 4h

Now, solving for T from Equation 5.9a gives

T =

= 

Qd

R(ln DT  ln D0 ) 148,000 J/mol

(8.31 J/mol-K)  ln (5.79  1011 m 2 /s)  ln (2.3  10 5 m 2 /s)    = 1381 K = 1108C

5.35 (a) Calculate the diffusion coefficient for magnesium in aluminum at 450°C. (b) What time will be required at 550°C to produce the same diffusion result (in terms of concentration at a specific point) as for 15 h at 450°C? Solution (a) We are asked to calculate the diffusion coefficient for Mg in Al at 450C. From Table 5.2, for this diffusion system D0 = 1.2  104 m2/s Qd =130,000 J/mol Thus, from Equation 5.8

 Q  D = D0 exp   d   RT    130,000 J/mol = (1.2  104 m 2 /s) exp    (8.31 J/mol-K)(450  273 K)  

 4.81  1014 m 2 /s (b) This portion of the problem calls for the time required at 550C to produce the same diffusion result as for 15 h at 450C. Equation 5.7 is employed as

D450t450 = D550t550 Now, from Equation 5.8 the value of the diffusion coefficient at 550C is calculated as

  130,000 J/mol D550 = (1.2  10 4 m 2 /s) exp     (8.31 J/mol-K)(550  273 K) 

 6.67  1013 m 2 /s Thus, solving for the diffusion time at 550C yields

t550 =

=

D450t450 D550

(4.81  1014 m 2 /s) (15h) = 1.08 h (6.67  1013 m 2 /s)

5.36 A copper–nickel diffusion couple similar to that shown in Figure 5.1a is fashioned. After a 500-h heat treatment at 1000°C (1273 K) the concentration of Ni is 3.0 wt% at the 1.0-mm position within the copper. At what temperature should the diffusion couple be heated to produce this same concentration (i.e., 3.0 wt% Ni) at a 2.0-mm position after 500 h? The preexponential and activation energy for the diffusion of Ni in Cu are 1.9 × 10 –4 m2/s and 230,000 J/mol, respectively. Solution In order to determine the temperature to which the diffusion couple must be heated so as to produce a concentration of 3.0 wt% Ni at the 2.0-mm position, we must first utilize Equation 5.6b with time t being a constant. That is, because time (t) is a constant, then

x2 = constant D Or 2 x1000 x2 = T D1000 DT

Now, solving for DT from this equation, yields

x2 D DT = T 1000 2 x1000 and incorporating into this expressions the temperature dependence of D1000 utilizing Equation 5.8, yields

 x   D exp   QRT   2 T

DT =

=

d

0

2 x1000



(2 mm)2  (1.9  104 m 2 /s)exp  

  230,000 J/mol  (8.31 J/mol-K)(1273 K)  

(1 mm)2

 2.74  1013 m 2 /s We now need to find the temperature T at which D has this value. This is accomplished by rearranging Equation 5.9a and solving for T as

T=

=

Qd

R (ln D0  ln D) 230,000 J/mol

(8.31 J/mol-K)  ln (1.9  104 m 2 /s)  ln (2.74  1013 m 2 /s)    = 1360 K = 1087C

5.37 A diffusion couple similar to that shown in Figure 5.1a is prepared using two hypothetical metals A and B. After a 20-h heat treatment at 800°C (and subsequently cooling to room temperature) the concentration of B in A is 2.5 wt% at the 5.0-mm position within metal A. If another heat treatment is conducted on an identical diffusion couple, but at 1000°C for 20 h, at what position will the composition be 2.5 wt% B? Assume that the preexponential and activation energy for the diffusion coefficient are 1.5 × 10 –4 m2/s and 125,000 J/mol, respectively. Solution In order to determine the position within the diffusion couple at which the concentration of A in B is 2.5 wt %, we must employ Equation 5.6b with t constant. That is

x2 = constant D Or 2 x800 x2 = 1000 D800 D1000

It is first necessary to compute values for both D800 and D1000; this is accomplished using Equation 5.8 as follows:

  125,000 J/mol D800 = (1.5  10 4 m 2 /s) exp     (8.31 J/mol-K)(800  273 K) 

1.22  1010 m 2 /s

  125,000 J/mol D1000 = (1.5  104 m 2 /s) exp     (8.31 J/mol-K)(1000  273 K) 

1.11  109 m 2 /s Now, solving the above expression for x1000 yields

x1000 = x800

= (5 mm)



D1000 D800

1.11  109 m2 /s

1.22  1010 m2 /s

= 15.1 mm

5.38  Consider the diffusion of some hypothetical metal Y into another hypothetical metal Z at 950 C; after 10 h the concentration at the 0.5 mm position (in metal Z) is 2.0 wt% Y.  At what position will the concentration also be 2.0 wt% Y after a 17.5 h heat treatment again at 950 C?  Assume preexponential and activation energy values of 4.3  10-4 m2/s and 180,000 J/mol, respectively, for this diffusion system. Solution In order to determine the position within this diffusion system at which the concentration of X in Y is 2.0 wt% after 17.5 h, we must employ Equation 5.6b with D constant (since the temperature is constant). (Inasmuch as D is constant it is not necessary to employ preexponential and activation energy values cited in the problem statement.) Under these circumstances, Equation 5.6b takes the form

x2 = constant t Or

x12 x22 = t1 t2 If we assume the following: x1 = 0.5 mm t1 = 10 h t2 = 17.5 h Now upon solving the above expression for x2 and incorporation of these values we have

x2 =

x12t2 t1

(0.5 mm) 2 (17.5 h) 10 h = 0.66 mm

5.39  A diffusion couple similar to that shown in Figure 5.1a is prepared using two hypothetical metals R and S.  After a 2.5­h heat treatment at 750 C the concentration of R is 4 at% at the 4­mm position within S.  Another heat treatment is conducted on an identical diffusion couple at 900 C and the time required to produce this same diffusion result (viz., 4 at% R at the 4­mm position within S) is 0.4 h.  If it is known that the diffusion coefficient at 750C is 2.6  10-17 m2/s determine the activation energy for the diffusion of R in S. Solution In order to determine the activation energy for this diffusion system it is first necessary to compute the diffusion coefficient at 900C.  Inasmuch as x is the same for both heat treatments, Equation 5.6b takes the form Dt = constant Or that

D750t750  D900t900 It is possible to solve for

D900

inasmuch as values for the other parameters are provided in the problem statement;

i.e.,

t750 = 2.5 h D750

= 2.6  10-17 m2/s

t900 = 0.4 h Solving for

D900

from the above equation leads to

D900 

D750 t750 t900

(2.6  1017 m 2 /s)(2.5 h) 0.4 h 1.6  1016 m2/s

Inasmuch as we know the values of D at both 750C and 900C—viz.,

D750 = 2.6  10-17 m2/s D900 = 1.6  10-16 m2/s

it is possible to solve for the activation energy Qd using the following equation, which is derived in Example Problem 5.5. In this expression, if we assign

D750 D1 =

and

D900 D2

=

, then the activation energy is equal to

 log D  log D  1 2 Qd  2.3R  1 1      T T  1 2  

 log(2.6  10 17 m 2 /s)  log(1.6  1016 m 2 /s)    (2.3)(8.31 J/mol i K)  1 1      (750  273 K) (900  273 K)   =120,700 J/mol

5.40 The outer surface of a steel gear is to be hardened by increasing its carbon content; the carbon is to be supplied from an external carbon-rich atmosphere maintained at an elevated temperature. A diffusion heat treatment at 600°C (873 K) for 100 min increases the carbon concentration to 0.75 wt% at a position 0.5 mm below the surface. Estimate the diffusion time required at 900°C (1173 K) to achieve this same concentration also at a 0.5mm position. Assume that the surface carbon content is the same for both heat treatments, which is maintained constant. Use the diffusion data in Table 5.2 for C diffusion in α-Fe. Solution In order to compute the diffusion time at 900C to produce a carbon concentration of 0.75 wt% at a position 0.5 mm below the surface we must employ Equation 5.6b with position constant; that is Dt = constant since x is a constant (0.5 mm). This means that

D600t600 = D900t900 In addition, it is necessary to compute values for both D600 and D900 using Equation 5.8. From Table 5.2, for the  diffusion of C in -Fe, Qd = 87,400 J/mol and D0 = 1.1  10 6 m2/s. Therefore,

  87,400 J/mol D600 = (1.1  10 6 m 2 /s) exp     (8.31 J/mol-K)(600  273 K) 

6.45  1012 m 2 /s

  87,400 J/mol D900 = (1.1  10 6 m 2 /s) exp    (8.31 J/mol-K)(900  273 K)  

1.40  1010 m 2 /s Now, solving the original equation for t900 gives

t900 =

=

(6.45

D600t600 D900

 1012 m 2 /s) (100 min) 1.40  1010 m 2 /s

= 4.61 min

5.41 An FCC iron–carbon alloy initially containing 0.10 wt% C is carburized at an elevated temperature and in an atmosphere in which the surface carbon concentration is maintained at 1.10 wt%. If after 48 h the concentration of carbon is 0.30 wt% at a position 3.5 mm below the surface, determine the temperature at which the treatment was carried out. Solution This problem asks us to compute the temperature at which a nonsteady-state 48 h diffusion anneal was carried out in order to give a carbon concentration of 0.30 wt% C in FCC Fe at a position 3.5 mm below the surface. From Equation 5.5

 Cx  C0 0.30  0.10 x  = = 0.2000 = 1  erf   Cs  C0 1.10  0.10  2 Dt  Or

x 

erf 

 = 0.8000

 2 Dt 

x Now it becomes necessary, using the data in Table 5.1 and linear interpolation, to determine the value of Thus z

erf (z)

0.90

0.7970

y

0.8000

0.95

0.8209

y  0.90 0.8000  0.7970 = 0.95  0.90 0.8209  0.7970 From which



y = 0.9063

Thus,

x 2 Dt

= 0.9063

And since t = 48 h (172,800 s) and x = 3.5 mm (3.5  103 m), solving for D from the above equation yields

2

Dt

.

D=

=

x2 (4t)(0.9063)2

(3.5  103 m )2 (4)(172,800 s)(0.821)

= 2.16  10 11 m 2 /s

Now, in order to determine the temperature at which D has the above value, we must employ Equation 5.9a; solving this equation for T yields

T=

Qd R (ln D0  ln D)

From Table 5.2, D0 and Qd for the diffusion of C in FCC Fe are 2.3  105 m2/s and 148,000 J/mol, respectively. Therefore

T=

148,000 J/mol (8.31 J/mol-K)  ln (2.3  105 m 2 /s)  ln (2.16  10 11 m 2 /s)    = 1283 K = 1010C

Diffusion in Semiconducting Materials 5.42 For the predeposition heat treatment of a semiconducting device, gallium atoms are to be diffused into silicon at a temperature of 1150C for 2.5 h.  If the required concentration of Ga at a position 2  m below the surface is 8  1023 atoms/m3, compute the required surface concentration of Ga.  Assume the following: (i)  The surface concentration remains constant (ii)  The background concentration is 2  1019 Ga atoms/m3 (iii)  Preexponential and activation energy values are 3.74  10-5 m2/s and 3.39 eV/atom, respectively. Solution This problem requires that we solve for the surface concentration, Cs of Equation 5.5 given the following: Cx = 8  1023 atoms/m3 C0 = 2  1019 atoms/m3 x = 2 m = 2  106 m T = 1150C t = 2.5 h = 9000 s D0 = 3.74  105 m2/s Qd = 3.39 eV/atom Equation 5.5 calls for a value of the diffusion coefficient D, which is determined at 1150C using Equation 5.8. Thus

 Q  D  D0 exp   d   RT 

  3.39 eV/atom  (3.74  105 m 2 /s)exp    5  (8.62  10 eV/atom K)(1150C + 273 K) 

 3.72  1017 m 2 /s Now it is required that we solve for Cs in Equation 5.5:

Cx  C0  x   1  erf  Cs  C0  2 Dt  

And solving for Cs from this expression and incorporation of values for all of the other parameters leads to

Cs  C0 +

 (2  1019 atoms/m 3 ) +

Cx  C0  x  1  erf   2 Dt  

(8  1023 atoms/m3 )  (2  1019 atoms/m 3 )   2  106 m  1  erf   2 (3.72  1017 m 2 /s)(9000 s)   

 (2  1019 atoms/m 3 ) +

(8  10 23 atoms/m 3 ) 1  erf (1.7283)

At this point it becomes necessary to conduct an interpolation—we know the z and need to determine the value of erf(z).  This interpolation is conducted using data found in Table 5.1 as follows: erf(z)

z

0.9838

1.7

erf(z)

1.7283

0.9891

1.8

1.8000  1.7283 0.9891  erf (z)  1.8000  1.7000 0.9891  0.9838 And solving this expression for erf(z) leads to

erf (z)  0.9853 Inserting this value into the above equation in which we are solving for Cs yields

Cs  (2  1019 atoms/m3 ) +

 (2  1019 atoms/m 3 ) +

(8  1023 atoms/m3 ) 1  erf (1.7283)

(8  1023 atoms/m3 ) 1  0.9853

 5.44  1025 Ga atoms/m3

5.43 Antimony atoms are to be diffused into a silicon wafer using both predeposition and drive-in heat treatments; the background concentration of Sb in this silicon material is known to be 2  1020 atoms/m3. The predeposition treatment is to be conducted at 900 C for 1 h; the surface concentration of Sb is to be maintained at a constant level of 8.0  1025 atoms/m3. Drive-in diffusion will be carried out at 1200 C for a period of 1.75 h. For the diffusion of Sb in Si, values of Qd and D0 are 3.65 eV/atom and 2.14  105 m2/s, respectively. (a) Calculate the value of Q0. (b) Determine the value of xj for the drive-in diffusion treatment. (c) Also, for the drive-in treatment, compute the position x at which the concentration of Sb atoms is 5  23

3

10 /m . Solution (a) For this portion of the problem we are asked to determine the value of Q0. This is possible using Equation 5.12. However, it is first necessary to determine the value of D for the predeposition treatment [Dp at Tp = 900°C (1173 K)] using Equation 5.8. Thus

 Q  Dp  D0 exp   d   kTp  3.65 eV    (2.14  10 5 m 2 /s)exp    5 (8.62  10 eV/atom K)(1173 K)  

 4.5  10 21 m 2 /s The value of Q0 is determined (using Equation 5.12) as follows:

Q0  2Cs

 (2)(8.0  1025 atoms/m3 )

Dptp

(4.5  1021 m 2 /s)(1 h)(60 min /h)(60 s/min) 

17 2 = 3.63  10 atoms/m

(b) Computation of the junction depth requires that we use Equation 5.13. However, before this is possible

it is necessary to calculate D at the temperature of the drive-in treatment [Dd at 1200°C (1473 K)]. Thus,

 Q  Dd  D0 exp   d   kTd    3.65 eV  (2.14  105 m 2 /s)exp    5  (8.62  10 eV/atom K)(1473 K ) 

 7.02  10 18 m 2 /s Now from Equation 5.13

xj   (4Ddtd )ln   C  B 



  (4)(7.02  10 

18

1/2

    Ddtd   

Q0

2

3.63  1017 atoms/m 2

m /s)(1.75 h)(60 min/h)(60 s/min) ln 

 

   (2  10 20 atoms/m 3 ) ( )(7.02  10 18 m 2 /s)(1.75 h)(60 min/h)(60 s/min)  

 1.23  106 m  1.23 m (c) For a concentration of 5  1023 Sb atoms/m3 for the drive-in treatment, we compute the value of x using Equation 5.11. However, it is first necessary to manipulate Equation 5.11 so that x is the dependent variable. Taking natural logarithms of both sides leads to

x2   Ddtd   4Ddtd Q0

lnC(x,t)  ln  

Now, rearranging and solving for x leads to

 

Q0

 

1/2

  x   (4Ddtd ) ln   C(x,t)  Ddtd     Now, incorporating values for Q0 and Dd determined above and taking C(x,t) = 5  1023 Sb atoms/m3 yields

1/2

x   (4)(7.02  10 

18

)(6300)ln 

3.63  1017

   

 (5  1023 ) ( )(7.02  1018 )(6300)     

 3.43  107 m  0.343 m

1/2

5.44 Indium atoms are to be diffused into a silicon wafer using both predeposition and drive-in heat treatments; the background concentration of In in this silicon material is known to be 2  1020 atoms/m3. The drivein diffusion treatment is to be carried out at 1175 C for a period of 2.0 h, which gives a junction depth x j of 2.35 m. Compute the predeposition diffusion time at 925 C if the surface concentration is maintained at a constant level of 2.5  1026 atoms/m3. For the diffusion of In in Si, values of Q d and D0 are 3.63 eV/atom and 7.85  105 m2/s, respectively. Solution This problem asks that we compute the time for the predeposition heat treatment for the diffusion of In in Si. In order to do this it is first necessary to determine the value of Q0 from Equation 5.13. However, before doing this we must first calculate Dd, using Equation 5.8. Therefore

 Q  Dd  D0 exp   d   kTd  3.63 eV    (7.85  10 5 m 2 /s)exp    5  (8.62  10 eV/atom K)(1175C  273 K) 

 1.84  10 17 m 2 /s Now, solving for Q0 in Equation 5.13 leads to

Q0  CB  Ddtd exp 

x2j 

  4Ddtd  

In the problem statement we are given the following values: CB = 2  1020 atoms/m3 td = 2 h (7,200 s) xj = 2.35 m = 2.35  10-6 m Therefore, incorporating these values into the above equation yields

  (2.35  10 6 m)2 Q0   (2  10 20 atoms/m 3 ) ( )(1.84  10 17 m 2 /s)(7, 200 s)  exp   17 2    (4)(1.84  10 m /s)(7, 200 s) 

 4.33  1018 atoms/m 2 We may now compute the value of tp using Equation 5.12. However, before this is possible it is necessary to determine Dp (at 925°C) using Equation 5.8. Thus

3.63 eV   Dp  (7.85  10 5 m 2 /s)exp    5  (8.62  10 eV/atom K)(925C  273 K) 

 4.25  10 20 m 2 /s Now, solving for tp in Equation 5.12 we get

tp 

 Q02 4Cs2 Dp

And incorporating the value of Cs provided in the problem statement (2  1025 atoms/m3) as well as values for Q0 and Dp determined above, leads to

tp 

 4.33  1018 atoms/m 2

2

2

(4) 2.5  10 26 atoms/m 3 (4.25  10 20 m 2 /s)

 5.54  10 3 s  92.3 min  1.53 h

DESIGN PROBLEMS Fick's First Law 5.D1 It is desired to enrich the partial pressure of hydrogen in a hydrogen–nitrogen gas mixture for which the partial pressures of both gases are 0.1013 MPa (1 atm). It has been proposed to accomplish this by passing both gases through a thin sheet of some metal at an elevated temperature; inasmuch as hydrogen diffuses through the plate at a higher rate than does nitrogen, the partial pressure of hydrogen will be higher on the exit side of the sheet. The design calls for partial pressures of 0.051 MPa (0.5 atm) and 0.01013 MPa (0.1 atm), respectively, for hydrogen and nitrogen. The concentrations of hydrogen and nitrogen (C H and CN, in mol/m3) in this metal are functions of gas partial pressures (p H2 and pN2, in MPa) and absolute temperature and are given by the following expressions:

 27,800 J/mol  CH  2.5  103 pH exp    2 RT  

(5.16a)

 37,600 J/mol  CN  2.75  103 pN exp    2 RT  

(5.16b)

Furthermore, the diffusion coefficients for the diffusion of these gases in this metal are functions of the absolute temperature as follows:

 13,400 J/mol  DH (m 2 /s)  1.4  10 7 exp    RT  

(5.17a)

 76,150 J/mol  DN (m 2 /s) = 3.0  107 exp    RT  

(5.17b)

Is it possible to purify hydrogen gas in this manner? If so, specify a temperature at which the process may be carried out, and also the thickness of metal sheet that would be required. If this procedure is not possible, then state the reason(s) why. Solution Since this situation involves steady-state diffusion, we employ Fick's first law, Equation 5.2. Inasmuch as the partial pressures on the high-pressure side of the sheet are the same, and the pressure of hydrogen on the low pressure side is 5 times that of nitrogen, and concentrations are proportional to the square root of the partial pressure, the diffusion flux of hydrogen, JH, is the square root of 5 times the diffusion flux of nitrogen JN--i.e.

JH 

5JN

Let us begin by producing expressions for the diffusion flux of both hydrogen and nitrogen, and then use them to satisfy the above equation. Fick's first law describing the flux of hydrogen, JH, is as follows:

J H   DH

CH x

  1  13,400 J/mol   (1.4  107 )  exp     C (Lo)  CH (Hi)    RT  x     H 

 

where

CH (Lo)

and

CH (Hi)

designate values of the concentrations of hydrogen on low and high pressure sides of

the plate. Expressions for these two parameters, as determined using Equation 5.16a, are as follows:

  27,800 J/mol   CH (Lo)  (2.5  103 )( 0.051 MPa )  exp     RT       27,800 J/mol   CH (Hi)  (2.5  103 )( 0.1013 MPa )  exp     RT    

C (Lo)  CH (Hi) Now, the expression for H may be written as follows:   27,800 J/mol   CH (Lo)  CH (Hi)  (2.5  103 )( 0.051 MPa  0.1013 MPa )  exp     RT     Hence, the expression for JH reads as follows

   1  13,400 J/mol    27,800 J/mol   3 J H   (1.4  107 )  exp    (2.5  10 )( 0.051 MPa  0.1013 MPa )  exp       RT RT  x         A Fick's first law expression for the diffusion flux of nitrogen may be formulated in a similar manner, which reads as follows:

J N   DN

CN x

   1  76,150 J/mol    37,600 J/mol   3 (3.0  107 )  exp    (2.75  10 )( 0.01013 MPa  0.1013 MPa )  exp       RT RT  x        

 

And, finally, as noted above, we want to equate these two expressions such that they satisfy the following relationship:

JH 

5JN

and then solve this relationship for the temperature T (taking the value of R to be 8.31 J/mol-K). Following through this procedure results in a temperature of T = 3467 K which value is extremely high (surely above the vaporization point of most metals). Thus, such a diffusion process is not possible.

5.D2 A gas mixture is found to contain two diatomic A and B species (A 2 and B2), the partial pressures of both of which are 0.1013 MPa (1 atm). This mixture is to be enriched in the partial pressure of the A species by passing both gases through a thin sheet of some metal at an elevated temperature. The resulting enriched mixture is to have a partial pressure of 0.051 MPa (0.5 atm) for gas A and 0.0203 MPa (0.2 atm) for gas B. The concentrations of A and B (CA and CB, in mol/m3) are functions of gas partial pressures (p A2 and pB2, in MPa) and absolute temperature according to the following expressions:

 20,000 J/mol  CA  1.5  103 pA exp    2 RT  

(5.18a)

 27,000 J/mol  CB  2.0  103 pB exp    2 RT  

(5.18b)

Furthermore, the diffusion coefficients for the diffusion of these gases in the metal are functions of the absolute temperature as follows:

 13,000 J/mol  DA (m 2 /s)  5.0  107 exp    RT  

(5.19a)

 21,000 J/mol  DB (m 2 /s)  3.0  106 exp    RT  

(5.19b)

Is it possible to purify the A gas in this manner? If so, specify a temperature at which the process may be carried out, and also the thickness of metal sheet that would be required. If this procedure is not possible, then state the reason(s) why. Solution Since this situation involves steady-state diffusion, we employ Fick's first law, Equation 5.2. Inasmuch as the partial pressures on the high-pressure side of the sheet are the same, and the pressure of A 2 on the low pressure side is 2.5 times that of B 2, and concentrations are proportional to the square root of the partial pressure, the diffusion flux of A, JA, is the square root of 2.5 times the diffusion flux of nitrogen JB--i.e.

JA =

2.5 J B

Let us begin by producing expressions for the diffusion flux of both A and B, and then use them to satisfy the above equation. Fick's first law describing the flux of A, JA, is as follows:

J A   DA

CA x

  1  13,000 J/mol   (5.0  107 )  exp     C (Lo)  CA (Hi)    RT  x     A 

 

where

CA (Lo)

and

CA (Hi)

designate values of the concentrations of species A on low and high pressure sides of

the plate, respectively. Expressions for these two parameters, as determined using Equation 5.18a, are as follows:

  20,000 J/mol   CA (Lo)  (1.5  103 )( 0.051 MPa )  exp     RT       20,000 J/mol   CA (Hi)  (1.5  103 )( 0.1013 MPa )  exp     RT    

C (Lo)  CA (Hi) Now, the expression for A may be written as follows:   20,000 J/mol   CA (Lo)  CA (Hi)  (1.5  103 )( 0.051 MPa  0.1013 MPa )  exp     RT     Hence, the expression for JA reads as follows

   1   13,000 J/mol    20,000 J/mol   3 J A   (5.0  107 )  exp    (1.5  10 )( 0.051 MPa  0.1013 MPa )  exp       RT RT  x         An expression for the diffusion flux for species B may be formulated in a similar manner, which reads as follows:

J B   DB

CB x

   1  21,000 J/mol    27,000 J/mol   3 (3.0  106 )  exp    (2.0  10 )( 0.0203 MPa  0.1013 MPa )  exp       RT RT  x        

 

And, finally, as noted above, we want to equate these two expressions such that they satisfy the following relationship:

JA =

2.5 J B

and then solve this relationship for the temperature T (taking the value of R to be 8.31 J/mol-K). Following through this procedure results in a temperature of T = 568 K (295C) Thus, this purification process is possible, which may be carried out at 568 K; furthermore, it is independent of sheet thickness.

Fick's Second Law—Nonsteady-State Diffusion 5.D3 The wear resistance of a steel shaft is to be improved by hardening its surface by increasing the nitrogen content within an outer surface layer as a result of nitrogen diffusion into the steel; the nitrogen is to be supplied from an external nitrogen-rich gas at an elevated and constant temperature. The initial nitrogen content of the steel is 0.0025 wt%, whereas the surface concentration is to be maintained at 0.45 wt%. For this treatment to be effective, a nitrogen content of 0.12 wt% must be established at a position 0.45 mm below the surface. Specify an appropriate heat treatment in terms of temperature and time for a temperature between 475°C and 625°C. The preexponential and activation energy for the diffusion of nitrogen in iron are 5 × 10 –7 m2/s and 77,000 J/mol, respectively, over this temperature range. Solution In order to specify time-temperature combinations for this nonsteady-state diffusion situation, it is necessary to employ Equation 5.5, utilizing the following values for the concentration parameters: C0 = 0.0025 wt% N Cs = 0.45 wt% N Cx = 0.12 wt% N Therefore, Equation 5.5

Cx  C0  x  = 1  erf  Cs  C0  2 Dt   takes the form

Cx  C0 0.12  0.0025 = Cs  C0 0.45  0.0025 

x   2 Dt  

= 0.2626 = 1  erf  Thus

1  0.2626 = 0.7374 = erf 

x 

 2 Dt  

Using linear interpolation and the data presented in Table 5.1

z

erf (z)

0.7500

0.7112

y

0.7374

0.8000

0.7421

0.7374  0.7112 y  0.7500 = 0.7421  0.7112 0.8000  0.7500 From which

 y=

x

4

The problem stipulates that x = 0.45 mm = 4.5  10

= 0.7924

2 Dt

m. Therefore

4.5  104 m 2 Dt

= 0.7924

Which leads to

Dt  8.06  108 m 2 Furthermore, the diffusion coefficient depends on temperature according to Equation 5.8; and, as stipulated in the 7

problem statement, D0 = 5  10

m2/s and Qd = 77,000 J/mol. Hence

 Q  Dt = D0exp   d (t)= 8.06  10-8 m 2  RT 

(5.0

 77,000 J/mol  8 2  107 m 2 /s) exp    (t)  8.06  10 m  (8.31 J/mol-K)(T) 

And solving for the time t

t (in s) =

0.161 9265.9  exp   T    

Thus, the required diffusion time may be computed for some specified temperature (in K). Below are tabulated t values for three different temperatures that lie within the range stipulated in the problem.

Temperature (C)

s

Time h

500

25,860

7.2

550

12,485

3.5

600

6,550

1.8

5.D4 The wear resistance of a steel gear is to be improved by hardening its surface, as described in Design Example 5.1. However, in this case the initial carbon content of the steel is 0.15 wt%, and a carbon content of 0.75 wt% is to be established at a position 0.65 mm below the surface. Furthermore, the surface concentration is to be maintained constant, but may be varied between 1.2 and 1.4 wt% C. Specify an appropriate heat treatment in terms of surface carbon concentration and time, and for a temperature between 1000°C and 1200°C. Solution This is a nonsteady-state diffusion situation; thus, it is necessary to employ Equation 5.5, utilizing values/value ranges for the following parameters: C0 = 0.15 wt% C 1.2 wt% C  Cs  1.4 wt% C Cx = 0.75 wt% C x = 0.65 mm 1000ºC  T  1200ºC Let us begin by assuming a specific value for the surface concentration within the specified range—say 1.2 wt% C. Therefore, Equation 5.5 takes the form

Cx  C0 0.75  0.15 = Cs  C0 1.20  0.15 

x 

= 0.5714 = 1  erf 

 2 Dt  

Thus

1  0.5714 = 0.4286 = erf 

x 

 2 Dt  

Using linear interpolation and the data presented in Table 5.1 z

erf (z)

0.4000

0.4284

y

0.4286

0.4500

0.4755

0.4286  0.4284 y  0.4000 = 0.4755  0.4284 0.4500  0.4000 from which

y=

x 2 Dt

= 0.4002

The problem statement stipulates that x = 0.65 mm = 6.5  104 m. Therefore

6.5  10 4 m 2 Dt

= 0.4002

Which leads to

Dt = 6.59  107 m 2 Furthermore, the diffusion coefficient depends on temperature according to Equation 5.8; and, as noted in Design Example 5.1, D0 = 2.3  105 m2/s and Q = 148,000 J/mol. Hence d

 Q  Dt = D0 exp   d (t)= 6.59  10-7 m 2  RT 

 (2.3

 148,000 J/mol  7 2  105 m 2 /s) exp    (t)  6.59  10 m (8.31 J/mol-K)(T)  

And solving for the time t

t (in s) =

2.86  10 2  17,810  exp   T   

Thus, the required diffusion time may be computed for some specified temperature (in K). Below are tabulated t values for three different temperatures that lie within the range stipulated in the problem.

Temperature (C)

Time s

h

1000

34,100

9.5

1100

12,300

3.4

1200

5,100

1.4

Now, let us repeat the above procedure for two other values of the surface concentration, say 1.3 wt% C and 1.4 wt % C. Below is a tabulation of the results, again using temperatures of 1000C, 1100C, and 1200C.

Cs (wt% C)

1.3

1.4

Temperature (C)

Time s

h

1000

26,700

7.4

1100

9,600

2.7

1200

4,000

1.1

1000

21,100

6.1

1100

7,900

2.2

1200

1,500

0.9

Diffusion in Semiconducting Materials 5.D5 One integrated circuit design calls for the diffusion of aluminum into silicon wafers; the background concentration of Al in Si is 1.75  1019 atoms/m3. The predeposition heat treatment is to be conducted at 975 C for 1.25 h, with a constant surface concentration of 4  1026 Al atoms/m3. At a drive-in treatment temperature of 1050C, determine the diffusion time required for a junction depth of 1.75 m. For this system, values of Q d and D0 are 3.41 eV/atom and 1.38  104 m2/s, respectively. Solution This problem asks that we compute the drive-in diffusion time for aluminum diffusion in silicon. Values of parameters given in the problem statement are as follows: CB = 1.75  1019 atoms/m3 Cs = 4  1026 atoms/m3 xj = 1.75 m = 1.75  106 m Tp = 975C = 1248 K Td = 1050C = 1323 K tp = 1.25 h = 4500 s Qd = 3.41 eV/atom D0 = 1.38  104 m2/s

It is first necessary to determine the value of Q0 using Equation 5.12. But before this is possible, the value of Dp at 975°C must be computed with the aid of Equation 5.8. Thus,

 Q  Dp  D0 exp   d   kTp 

  3.41 eV  (1.38  104 m 2 /s)exp     (8.62  105 eV/atom K)(975C  273 K) 

 2.36  10 18 m 2 /s

Now for the computation of Q0 using Equation 5.12:

Q0  2Cs

 (2)(4  1026 atoms/m3 )

Dptp

(2.36  1018 m 2 /s)(1.25 h)(60 min/h)(60 s/min) 

 4.65  1019 atoms/m 2 We now desire to calculate td in Equation 5.13. Algebraic manipulation and rearrangement of this expression leads to

x2j 

Q0   4Ddtd  CB  Ddtd 

exp 

At this point it is necessary to determine the value of Dd (at 1050°C). This possible using Equation 5.8 as follows:

  3.41 eV Dd  (1.38  104 m 2 /s)exp    5  (8.62  10 eV/atom K)(1050C  273 K) 

 1.426  1017 m 2 /s And incorporation of values of all parameters except td in the expression cited above—i.e.,

x2j 

Q0   4Ddtd  CB  Ddtd 

exp  yields

 (1.75  10 6 m)2 4.65  1019 atoms/m 2   17 m 2 /s)t  (4)(1.426  10 (1.75  1019 atoms/m 3 ) ( )(1.426  10 17 m 2 /s)td d  

exp 

which expression reduces to

 5.37  10 4 s  3.96  108 s1/2   td td  

exp 

Solving for td is this expression is not a simple matter. One possibility is to use a graphing technique. Let us take the logarithm of both sides of the above equation, which gives

 3.96  108 s1/2  5.37  104 s  ln   td   td  Now if we plot the terms on both left and right hand sides of this equation versus td, the value of td at the point of intersection of the two resulting curves is correct answer. Below is such a plot:

As noted, the two curves intersect at about 3400 s, which corresponds to td = 0.94 h.

FUNDAMENTALS OF ENGINEERING QUESTIONS AND PROBLEMS 5.1FE Atoms of which of the following elements will diffuse most rapidly in iron? (A) Mo

(C) Cr

(B) C

(D) W Solution

The correct answer is B. Carbon atoms diffuse most rapidly because they are smaller than atoms of Mo, Cr, and W. Furthermore, diffusion of C in Fe is via an interstitial mechanism, whereas for Mo, Cr, and W the mechanism is vacancy diffusion.

5.2FE Calculate the diffusion coefficient for copper in aluminum at 600 C. Preexponential and activation energy values for this system are 6.5  10–5 m2/s and 136,000 J/mol, respectively. (A) 5.7  102 m2/s

(C) 4.7  1013 m2/s

(B) 9.4  1017 m2/s

(D) 3.9  102 m2/s

Solution We are asked to calculate the diffusion coefficient for Cu in Al at 600C, given values for D0 and Qd. This determination is possible using Equation 5.8 as follows:

 Q  D = D0 exp   d   RT    136, 000 J/mol = (6.5  10 5 m 2 /s)exp    (8.31 J/mol-K)(600  273 K)   = 4.7  1013 m2/s Therefore, the correct answer is C.

Comments

Copyright ©2017 KUPDF Inc.